Synthesis, structure and optical properties of two isotypic crystals, Na3MO4Cl (M=W, Mo)
Han, Shujuan; Bai, Chunyan; Zhang, Bingbing; Yang, Zhihua; Pan, Shilie; Journal of Solid State Chemistry 237 (2016) 14–18; doi:10.1016/j.jssc.2016.01.009

data_1561544
_publ_section_title
;
 Synthesis, structure and optical properties of two isotypic crystals,
 Na3MO4Cl (M=W, Mo)
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              14
_journal_page_last               18
_journal_paper_doi               10.1016/j.jssc.2016.01.009
_journal_volume                  237
_journal_year                    2016
_chemical_formula_sum            'Cl Na3 O4 W'
_chemical_formula_weight         352.27
_space_group_IT_number           129
_space_group_name_Hall           '-P 4a 2a'
_space_group_name_H-M_alt        'P 4/n m m :2'
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_H-M   'P 4/n m m :2'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   7.5181(15)
_cell_length_b                   7.5181(15)
_cell_length_c                   5.360(2)
_cell_measurement_reflns_used    1143
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.31
_cell_measurement_theta_min      3.80
_cell_volume                     302.96(14)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0246
_diffrn_reflns_av_sigmaI/netI    0.0148
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       6
_diffrn_reflns_limit_l_min       -6
_diffrn_reflns_number            1733
_diffrn_reflns_theta_full        27.31
_diffrn_reflns_theta_max         27.31
_diffrn_reflns_theta_min         3.80
_exptl_absorpt_coefficient_mu    19.644
_exptl_absorpt_correction_T_max  0.7455
_exptl_absorpt_correction_T_min  0.4308
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   Face-indexed
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    3.862
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       bolck
_exptl_crystal_F_000             312
_exptl_crystal_size_max          0.19
_exptl_crystal_size_mid          0.18
_exptl_crystal_size_min          0.10
_refine_diff_density_max         0.559
_refine_diff_density_min         -0.819
_refine_diff_density_rms         0.122
_refine_ls_extinction_coef       0.0305(15)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.192
_refine_ls_matrix_type           full
_refine_ls_number_parameters     20
_refine_ls_number_reflns         217
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.192
_refine_ls_R_factor_all          0.0104
_refine_ls_R_factor_gt           0.0099
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0144P)^2^+0.1036P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0275
_refine_ls_wR_factor_ref         0.0279
_reflns_number_gt                207
_reflns_number_total             217
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            JSSC-2016-237-14.cif
_cod_data_source_block           11
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_exptl_absorpt_correction_type' value 'Numerical' was
changed to 'numerical' in accordance with the built-in table derived
from the CIF Core dictionary named 'cif_core.dic' version 2.4.5 last
updated on 2014-11-21.

data item '_symmetry_cell_setting' value 'Tetragonal' was changed to
'tetragonal' in accordance with the built-in table derived from the
CIF Core dictionary named 'cif_core.dic' version 2.4.5 last updated
on 2014-11-21.

Automatic conversion script
Id: cif_fix_values 8369 2020-08-20 11:38:08Z andrius 
;
_cod_original_sg_symbol_H-M      P4/nmm
_cod_database_code               1561544